Composites Design and Analysis. Stress Strain Relationship


 Millicent O’Neal’
 10 months ago
 Views:
Transcription
1 Composites Design and Analysis Stress Strain Relationship
2 Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines Design Data Quality Assurance
3 The design/analysis engineer should be able to determine for the following question: How do composite laminates behave under load? Which composite material should be used? What are the guidelines for design and the analysis methods? What design data is required and how is it obtained? Can the composite product be fabricated easily? How can the quality of the composite product be assured? The purpose of the material presented here is to introduce the reader to the principles of the mechanical behavior of thin laminates (how laminates behave under loads). This includes both symmetric and unsymmetric laminates relative to the midplane, with both inplane and flexural loads. Also included are the effects of temperature and moisture, and laminate strength. A liberal use is made of flow charts for aids in analysis
4 Stress Strains Relationships in Lamina (1) The lamina is homogeneous, orthotropic and linearelastic (2) The lamina is in a state of plane stress (very thin), therefore, the stresses associated with the zdirection are negligible: σ z = τ xz = τ yz = 0
5 The normal strain in the xdirection for the lamina in Figure 2a is the sum of the normal strains in the xdirection for the laminae in Figures 2b, 2c and 2d: From Figure 2b, ε x = 0 x x From Figure 2c, E x = or εx = x Ex x y From Figure 2d, ν y = or εx = ν y ε y = ν y y Ey Consequently, the total normal strain in the xdirection is x νy y ε x = 0 + Ex Ey x y or ε x = νy Ex Ey
6 The normal strain in the ydirection for the lamina is determined from superposition as follows: From Figure 2b, ε y = 0 y x From Figure 2c, ν x = or εy = ν x ε x = ν x x Ex y y From Figure 2d, E y = or εy = y Ey Consequently, the total normal strain in the ydirection is or x + y y ε y = 0 ν x Ex E x y ε y = ν x + Ex Ey (2) The shear strain, which is independent of the normal strains, is determined as follows: s s From Figure 2b, E s = or εs = s Es From Figure 2c, ε s = 0 From Figure 2d, ε s = 0 Therefore, the shear strain associated with the xy coordinate system is; ε s = s E s (3)
7 If we express Equations (1), (2) and (3) in matrix form, we have s y x = s y x x y y x E E E E E s y x = ss yy yx xy xx S S S S S s y x (4) Equation (4) may also be expressed as follows: s y x = s y x y y x y x y x x y y x x E E E E E s y x = ss yy yx xy xx Q Q Q Q Q s y x (5) [ε] = [C] [σ] [σ] = [M] [ε]
8 Elastic Constants x P σ x = P/A ε x ε y ν x = ε y / ε x lbs psi in/in in/in ν x = (average)
9 Elastic Constants y σ y vs ε y P σ y = P/A ε x ε y ν y = ε x / ε y lbs psi in/in in/in σ y (psi) 6000 E y = σ y / ε y = 3.05 x 10 6 psi ν y = (average) ε y (in/in)
10 Elastic Constants s P σ s = P/2A ε μ ε ν ε s = ε μ ε ν lbs psi in/in in/in in/in
11 Determination of Elastic Constants Type Material E x E y ν x E s ν f Specific gravity Typical thickness Type Material E x E y ν x E s t GPa GPa GPa meters T300/5208 Graphite/Epoxy T300/5208 Graphite/Epox y Msi Msi Msi inches B(4)/5505 Boron/Epoxy B(4)/5505 Boron/Epoxy AS/3501 Graphite/Epoxy Scotchply 1002 Glass/Epoxy AS/3501 Graphite/Epox y Kevlar 49/Epoxy Aramid/Epoxy Scotchply 1002 Glass/Epoxy Kevlar 49/Epoxy Aramid/Epoxy
12 Transformation of Stress and Strain
13 Area Stresses Stresses Forces
14 These three equilibrium equations may be combined in matrix form as follows:
15 The equations for the transformation of strain are the same as those for the transformation of stress:
16 Stress Strain Relationships in Global Coordinates Develop the relationship between the stresses and strains in global coordinates.
17 Stress Strain Relationships in Global Coordinates [σ xys ] = [Q xys ] [ε xys ] (1) [σ xys ] = [T] [ σ 126 ] (2) and [ε xys ] = [Ť] [ε 126 ] (3) Substitution of Equations (2) and (3) into (1) yields [T] [ σ 126 ] = [Q xys ] [Ť] [ε 126 ] (4) Pre multiplying both sides of Equation (4) by [T] 1 : [T] 1 [T] [σ 126 ] = [T] 1 [Q xys ] [Ť] [ε 126 ] (5) or [ σ 126 ] = [T] 1 [Q xys ] [Ť] [ε 126 ] (6) or = [T] 1 [Q xys ] [Ť] (7)
18 or = [Q 126 ] or [ σ 126 ] = [Q 126 ] [ε 126 ] where [Q 126 ] = [T] 1 [Q xys ] [Ť] Note that [T (+θ) ] 1 = [T ( θ) ] The elements of the matrix [Q 126 ] are as follows: Q 11 = Q xx cos 4 θ + 2 (Q xy + 2 Q ss ) sin 2 θ cos 2 θ + Q yy sin 4 θ Q 22 = Q xx sin 4 θ + 2 (Q xy + 2 Q ss ) sin 2 θ cos 2 θ + Q yy cos 4 θ Q 12 = Q 21 = (Q xx + Q yy 4Q ss ) sin 2 θ cos 2 θ + Q xy (sin 4 θ +cos 4 θ) Q 66 = (Q xx + Q yy 2 Q xy 2Q ss ) sin 2 θ cos 2 θ + Q ss (sin 4 θ +cos 4 θ) Q 16 = Q 61 = (Q xx Q xy 2Q ss ) sinθ cos 3 θ + (Q xy Q yy + 2Q ss ) sin 3 θ cosθ Q 26 = Q 62 = (Q xx Q xy 2Q ss ) sin 3 θ cosθ + (Q xy Q yy + 2Q ss ) sinθcos 3 θ
19 [Q 126 ] 1 [ σ 126 ] = [Q 126 ] 1 [Q 126 ] [ε 126 ] or [Q 126 ] 1 [ σ 126 ] = [ε 126 ] or [ε 126 ] = [Q 126 ] 1 [ σ 126 ] or [ε 126 ] = [S 126 ] [ σ 126 ] or The elements of the matrix [S 126 ] are as follows: S 11 = (Q 22 Q 66 Q 262 ) / S 12 = S 21 = (Q 16 Q 26 Q 12 Q 66 ) / S 16 = S 61 = (Q 12 Q 26 Q 22 Q 16 ) / S 22 = (Q 11 Q 66 Q 162 ) / S 26 = S 62 = (Q 12 Q 16 Q 11 Q 26 ) / S 66 = (Q 11 Q 22 Q 122 ) / where = Q 11 Q 22 Q Q 12 Q 26 Q 61 Q 22 Q 16 2 Q 66 Q 12 2 Q 11 Q 62 2
20 Summary: Lamina Analysis
21 The Symmetric Laminate with In Plane Loads A. Stress Resultants and Strains: The A
22 Relationship between strains and the stress resultants. Related by constants Aij Deriving expressions for these constants: Expression for is:
23 Expression for N 1: N 1 = (σ 1 ) 1 (h 1 h 2 ) + (σ 1 ) 2 (h 2 h 3 ) + (σ 1 ) 3 (h 3 h 4 ) + Substitute the expressions for stress:
24 Above equation can be rewritten as: Similarly for N2 and N6:
25 Above can be combined into matrix form as: Or Where A 11 = (Q 11 ) k t k A 12 = (Q 12 ) k t k A 16 = (Q 16 ) k t k A 22 = (Q 22 ) k t k A 26 = (Q 26 ) k t k A 66 = (Q 66 ) k t k
26 Example Determine the elements of [A] for a symmetric laminate of 6 layers: [0/45/90] s. The material of each lamina is Gr/Ep T300/5208 and t=0.005 = m 0 Lamina 90 Lamina Q 11 = Q xx = Q 11 = Q yy = Q 22 = Q yy = Q 22 = Q xx = Q 12 = Q xy = Q 12 = Q xy = Q 66 = Q ss = 7.17 Q 66 = Q ss = 7.17 Q 16 = 0 Q 16 = 0 Q 26 = 0 Q 26 = 0 Q 11 = Q xx cos 4 θ + 2 (Q xy + 2 Q ss ) sin 2 θ cos 2 θ + Q yy sin 4 θ Q 22 = Q xx sin 4 θ + 2 (Q xy + 2 Q ss ) sin 2 θ cos 2 θ + Q yy cos 4 θ Q 12 = Q 21 = (Q xx + Q yy 4 Q ss ) sin 2 θ cos 2 θ + Q xy (sin 4 θ + cos 4 θ) Q 66 = (Q xx + Q yy 2Q xy 2 Q ss ) sin 2 θ cos 2 θ + Q ss (sin 4 θ + cos 4 θ) Q 16 = Q 61 = (Q xx Q xy 2 Q ss ) sinθ cos 3 θ + (Q xy Q yy + 2 Q ss ) sin 3 θ cosθ Q 26 = Q 62 = (Q xx Q xy 2 Q ss ) sin 3 θ cosθ + (Q xy Q yy + 2 Q ss ) sinθ cos 3 θ Q 11 = 0.25 Q xx + 2 (Q xy + 2 Q ss ) (0.25) Q yy = 56.65
27 Q 22 = 0.25 Q xx + 2 (Q xy + 2 Q ss ) (0.25) Q yy = Q 12 = (Q xx + Q yy 4 Q ss ) (0.25) + Q xy (0.5) = Q 66 = (Q xx + Q yy 2 Q xy 2Q ss ) (0.25) + Q ss (0.25) = Q 16 = (Q xx Q xy 2 Q ss ) (0.25) + (Q xy Q yy +2 Q ss ) (0.25) = Q 26 = (Q xx Q xy 2 Q ss ) (0.25) + (Q xy Q yy +2 Q ss ) (0.25) = The Laminate A 11 = ( ) 2 = A 22 = ( ) 2 = A 12 = ( ) 2 = A 66 = ( ) 2 = A 16 = ( ) 2 = A 26 = ( ) 2 = GPa m
28 Equivalent Engineering Constants for the Laminate Equation for the composite laminate is Or [N] = [A] [ε] Matrix equation for a single orthotropic lamina or layer is Or [σ] = [M] [ε]
29 The properties of the single equivalent orthotropic layer can be determined from the following equation: [A] = [M] where h = laminate thickness or 1 A 11 = E1 1 A 12 = 2E1 1 A 66 = E 6 h h h 1 h A 22 = E 2 1 A 21 = h 1E Solving last equation, we have the following elastic constants for the single equivalent orthotropic layer: A11 A22 E 1 = (1 ) E 2 = (1 ) h A12 2 A11A 22 h A A A 22 1 h 12 E 6 = A 66 ν 1 = ν 2 = A A 22 A A 12 11
30 The equation for the composite laminate is or [ε] = [a] [N] where [a] = [A] 1 The equation for a single orthotropic lamina is or [ε] = [C] [σ]
31 The properties of the single equivalent orthotropic layer is determined by [a] h = [C] 1 2 or a 11 h = a 12 h = a 66 h = E E1 2 1 E 6 1 a 21 h = a 22 h = E 1 1 E 2 elastic constants for the single equivalent orthotropic layer: E 1 = 1 E 2 = E 66 = a11h 1 a22h 1 a66h a a 12 ν 1 = ν 2 = 11 a a 12 22
32 1) Cross Ply Laminates Special Cases:
33
34 Balanced Angle Ply Laminates:
35 Example: [0, 90] un symmetric cross ply, A 16 = A 26 = 0 [0, 90, 0] symmetric cross ply, A 16 = A 26 = 0 [+30, 30, 30, +30] symmetric balanced angle ply, A 16 = A 26 = 0 [+30, 30, +30, 30] un symmetric balanced angle ply, A 16 = A 26 = 0 [+30, 30, +30] symmetric un balanced angle ply, A 16, A 26 0
36 3) Quasi Isotropic Laminates: Has m ply groups spaced at ply orientations of 180/m degrees. Examples: [0/60/ 60]s m = 3 180/m = 60 [0/90/45/ 45]s m = 4 180/m = 45 [0/60/ 60/60/0/ 60]s m=3 180/m = 60 The modulus of the quasi isotropic laminate has the following properties: A 11 = A 22 A 16 = A 26 = 0 A 66 = (A 11 A 22 ) which is equivalent to G = 1 2 E 1 for an isotropic material.
37 Summary: Laminate Analysis
38 The Symmetric Laminate with Bending and Twisting Loads: The D Matrix M 1 and M 2 are bending moments per unit length M 6 is a twisting couple per unit length. The basic difference between in plane loading and flexural loading is that the strains are not the same in all layers of the laminate that has flexural loading.
39 The Symmetric Laminate with Bending and Twisting Loads: The D Matrix Stress Resultants and Curvatures: The D Matrix 1 2 d w dx ε x = (z ) = (z 2 ) = z K where ρ is the radius of curvature, and K is defined as the curvature. Note (from Figure 2) that z is positive and is negative. Thus ε x is positive, which is evident from inspection of the figure.
40 ε 1 = z = z K 1 ε 2 = z = z K 2 ε 6 = 2 z = z K 6 = z [ε 126 ] = z [K 126 ] where K 1, K 2 and K 6 are referred to as the curvatures [σ 126 ] = [Q 126 ] [ε 126 ] [σ 126 ] = z[q 126 ] [K 126 ] X w X w X X w K K K
41 The objective of this section is to determine the elements of the matrix which relates the flexural loads M 1, M 2, M 6 to the curvatures K 1, K 2, K 6 for a symmetric laminate. This matrix is defined as the D matrix: Furthermore, we wish to determine the relationship between the loads M 1, M 2, M 6 and the stresses and strains in a particular layer a distance z from the laminate mid plane.
42 The stress resultant M 1, which has units of pounds per inch of length in the 2 direction, is determined as follows: If we use the expression for σ 1 from Equation 5, M 1 becomes
43 After integration, M 1 becomes where k represents the k th layer and n is the number of layers. Similarly
44 If we combine above three equations, we get The elements of the D matrix are
45 B. Equivalent Engineering Constants for the Laminate with Flexural Loading A composite laminate may sometimes be modeled as an equivalent orthotropic single layer, as discussed in Section III B, with the D matrix as well as the A matrix. The objective here is to determine the elastic constants for this equivalent orthotropic layer, and to explain when it is appropriate to use them. The equation for the composite laminate is The equation for a single orthotropic layer is
46 The properties of the single equivalent orthotropic layer can be determined by equating the modulus of equation (1) with that of Equation (2): If we equate the individual elements of the left hand side of equation (3) with the corresponding elements on the right hand side, then solve for the elastic constants, we have
47 We model the structure with orthotropic plate elements to be used in a finite element program. The elastic constants of these equivalent orthotropic plate elements are determined from Equations (4). We take the results of the finite element program and determine M 1, M 2, and M 6 at the point we are interested in analyzing. Then we use the equations developed in Section II and IV to determine the stresses and strains in the various layers. This method is appropriate for laminates with D 16 = D 26 = 0 and flexural loading. For the more general cases in which D 16 and D 26 are not zero, this method is approximate and must be used with discretion. If the laminate loads are in plane rather than flexural, we should use the equivalent elastic constants derived in Section III B rather than those presented in this section. For laminates with many layers, the equivalent laminate elastic constants of Section III B and those presented here approach each other in value.
48 Cross Ply Laminates: C. Special Cases: All layers are either 0 or 90, which results in D 16 = D 26 = 0. This is sometimes called special orthotropic w. r. t. flexure. Balanced Angle Ply Laminates: There are only two orientations of the plies (same magnitude but opposite in sign) with an equal number of plies with positive and negative orientations. If for every layer at θ above the mid plane, there is an identical layer at θ below the mid plane, then D 16 = D 26 = 0. However, this does not produce a symmetric laminate and leads to coupling between mid plane strains and curvatures. If the laminate is symmetric then, D 16 and D 26 are not zero. However, as the number of layers approaches infinity, the terms D 16 and D 26 approach zero.
49 Example: [0, 90] un symmetric cross ply, A 16 = A 26 = D 16 = D 26 = 0 [0, 90, 0] symmetric cross ply, A 16 = A 26 = D 16 = D 26 = 0 [+30, 30, +30, 30] un symmetric balanced angle ply, A 16 = A 26 = D 16 = D 26 = 0 [+30, 30, 30, +30] symmetric balanced angle ply, A 16 = A 26 = 0, and D 16, D 26 0 [+30, 30, +30] symmetric un balanced angle ply, A 16, A 26 0, and D 16, D 26 0 [+30, 30] 4s or [+30, 30, +30, 30, +30, 30, +30, 30] s or 16 ply symmetric balanced angle ply, A 16 = A 26 = 0, and D 16, D 26 0
50 D. Summary: Laminate Analysis
51 Problems (Chapter IV) The stress in the upper 45 layer for the lamina shown are ρ x = 400 MPa, ρ y = 50 MPa, ρ s = 70 MPa. The thickness of each lamina is meters. Determine the loads (stress resultants M 1, M 2, M 6 ) that would cause these stresses. Use either metric or English units. The [D] matrix for this laminate is (metric): Verify the value for D 12.
52 V: The Symmetric Laminate with both In Plane and Flexural Loads We merely combine these two equations for the laminate shown in Figure 1; The strains of Equation 8, Section III A, must be interpreted as mid plane strains: ε 1o, ε 2o, ε 6o are the mid plane strains of the symmetric laminate K 1, K 2, K 6 are the laminate curvatures as discussed in Section IV A. The elements of the A matrix are defined by Equations (9), Section III A and he elements of the D matrix are defined by Equations 12, Section IV A.
53 Equation 1, Section IV A relates the curvatures K 1, K 2, K 6 and the strains ε 1, ε 2, ε 6 in a particular lamina for a symmetric laminate with flexural loading. For the laminate subjected to both flexural loading and inplane loading, the strains and stresses in a particular lamina must be written in terms of mid plane strains as well as the curvatures:
54 The quantities on the left hand side of Equation (2) are the strains in a particular lamina a distance z from the mid plane and are composed of two parts as shown. The strains [ε o 126] are produced by the in plane loads and the strains z [K 126 ] are produced by the flexural loads. This is shown in detail in Figure 2 for the strain component ε 1. The displacement of point a in the 1 direction is The strain in the 1 direction of point a is, by definition,
55 Summary: Laminate Analysis
56 We are given a set of allowable stresses in local coordinates (σ x, σ y, σ z ) for a particular lamina in a laminate and our objective is to calculate the allowable stress resultants. First, we must realize that we cannot solve for 6 unknowns by prescribing just 3 knowns. If we are given (σ x, σ y, σ z ) k, we can determine (ε x, ε y, ε z ) k, (ε 1, ε 2, ε 6 ) k, and (σ 1, σ 2, σ 6 ) k as shown by Figure 1. However, we can not determine (ε 1o, ε 2o, ε 6o,K 1, K 2, K 6 ) because we do not have 6 independent equations; Note that (ε 1, ε 2, ε 6 ) k and (σ 1, σ 2, σ 6 ) k are not independent. In fact, they are related by Equations (9) or (5). Thus we need to prescribe any 3 of the following 12 quantities: N 1, N 2, N 6, M 1, M 2, M 6, ε 1o, ε 2o, ε 6o, K 1, K 2, K 6. Now we may continue the solution and solve for the remaining unknowns. In summary: If we are given (N 1, N 2, N 6, M 1, M 2, M 6 ), we can solve for all other quantities. If we are given (ε 1o, ε 2o, ε 6o,K 1, K 2, K 6 ), we can solve for all other quantities. If we are given (ε x, ε y, ε z ) k, we must also be given the values for any 3 of the quantities in (1) or (2). Then we can proceed to solve for all other quantities.
57 Problems (Chapter V) A laminate consists of Graphite/Epoxy, T300/5208, layers as follows: [0, 45, 45, 90] s. The applied stress resultants are M 1 = 25 in lb/in, M 2 = 0, M 6 = 0, N 1 = 1500 lb/in, N 2 = 0, N 6 = 0. Determine the stresses (σ x, σ y, σ z ) midway between the upper and lower surface of the upper 45 lamina. Verify the values for elements A 22 and D 22.
58 VI: The Unsymmetrical Laminate If the laminate is symmetric, there is no coupling between mid plane strains and laminate curvatures, as illustrated by Equation (1) of Section V A. However, if the laminate is unsymmetric, coupling does exist as shown in Equation (1) below: The objective here is to derive the elements of the matrix that relates the in plane and bending stress resultants to the mid plane strains and laminate curvatures. We are especially interested in the B matrix of Equation (1).
59 Before we proceed with this derivation, recall the equations for the strains in the k th lamina, Equation (2) of Section V A: [ε 126 ] k = [ε o 126] + z [K 126 ] We obtain the expression for the strains in the k th lamina by substituting Equation (3) into Equation (9) of Section II D: [σ 126 ] k = [Q 126 ] k [ε 126 ] k [σ 126 ] k = [Q 126 ] k [ε o 126] + z [Q 126 ] k [K 126 ]
60 The expression for N 1 is determined as follows: Substitution of the expression for σ 1 from Equation (4) into equation (5) yields:
61 After integration, Equation (6) becomes: where n is the number of layers in the laminate and k refers to a particular layer. Similarly:
62 The expression for M 1 is: If we obtain the expression for σ 1 from Equation (4) and follow the procedure presented in Section IV A, we have Similarly,
63 If we combine Equations (8), (9) and (10), we have If we combine Equations (12), (13) and (14), we have
64 We now combine Equation (16) and (18) and the derivation is complete: Where A ij = (Q ij ) k (b k a k ) B ij = (Q ij ) k b 2 2 k a k 2 D ij = (Q ij ) k b 3 3 k a k 3 If the laminate is symmetric w. r. t. the mid plane, we see that B ij = 0, and the in plane quantities become uncoupled from the flexural quantities. Otherwise, there is coupling because of the existence of the B matrix. That is, in plane loads cause bending and twisting as well as in plane strains. Also, flexural loads cause in plane strains as well as bending and twisting.
65 Summary: Laminate Analysis
66
67
68 Problems (Chapter VI) A laminate consists of Graphite/Epoxy, T300/5208, layers as follows: [0, 45, 90]. The applied stress resultants are N 1 = 100 lb/in, N 2 = N 6 = M 1 = M 2 = M 6 = 0. Determine the stresses (σ x, σ y, σ z ) in the middle of the 90 lamina.
Chapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationStrain Transformation equations
Strain Transformation equations R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 8 Table of Contents 1. Stress transformation
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationOutline. Organization. Stresses in Beams
Stresses in Beams B the end of this lesson, ou should be able to: Calculate the maimum stress in a beam undergoing a bending moment 1 Outline Curvature Normal Strain Normal Stress Neutral is Moment of
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More informationChapter 12 Plate Bending Elements. Chapter 12 Plate Bending Elements
CIVL 7/8117 Chapter 12  Plate Bending Elements 1/34 Chapter 12 Plate Bending Elements Learning Objectives To introduce basic concepts of plate bending. To derive a common plate bending element stiffness
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationBALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS
7 th International LSDYNA Users Conference Penetration/Explosive BALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS ChianFong Yen Materials Sciences Corporation 5 Office Center Drive Fort Washington, PA
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationKirchhoff Plates: Field Equations
20 Kirchhoff Plates: Field Equations AFEM Ch 20 Slide 1 Plate Structures A plate is a three dimensional bod characterized b Thinness: one of the plate dimensions, the thickness, is much smaller than the
More informationSection Downloads. Section Downloads. Handouts & Slides can be printed. Other documents cannot be printed Course binders are available for purchase
Level II: Section 04 Simplified Method (optional) Section Downloads Section Downloads Handouts & Slides can be printed Version.0 Other documents cannot be printed Course binders are available for purchase
More informationMECE 3321: MECHANICS OF SOLIDS CHAPTER 5
MECE 3321: MECHANICS OF SOLIDS CHAPTER 5 SAMANTHA RAMIREZ TORSION Torque A moment that tends to twist a member about its longitudinal axis 1 TORSIONAL DEFORMATION OF A CIRCULAR SHAFT Assumption If the
More informationNote that W is the skin surface weight density in units of psf. An equivalent graph in terms of metric units is given in Appendix A.
VIBRATION RESPONSE OF A CYLINDRICAL SKIN TO ACOUSTIC PRESSURE VIA THE FRANKEN METHOD Revision H By Tom Irvine Email: tomirvine@aol.com September 16, 2008 Introduction The front end of a typical rocket
More informationFIXED BEAMS IN BENDING
FIXED BEAMS IN BENDING INTRODUCTION Fixed or builtin beams are commonly used in building construction because they possess high rigidity in comparison to simply supported beams. When a simply supported
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 1
MECE 3321 MECHANICS O SOLIDS CHAPTER 1 Samantha Ramirez, MSE WHAT IS MECHANICS O MATERIALS? Rigid Bodies Statics Dynamics Mechanics Deformable Bodies Solids/Mech. Of Materials luids 1 WHAT IS MECHANICS
More informationFlexible Pavement Stress Analysis
Flexible Pavement Stress Analysis Dr. Antonis Michael Frederick University Notes Courtesy of Dr. Christos Drakos, University of Florida Need to predict & understand stress/strain distribution within the
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationStresses and Strains in flexible Pavements
Stresses and Strains in flexible Pavements Multi Layered Elastic System Assumptions in Multi Layered Elastic Systems The material properties of each layer are homogeneous property at point A i is the same
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationExternal Work. When a force F undergoes a displacement dx in the same direction i as the force, the work done is
Structure Analysis I Chapter 9 Deflection Energy Method External Work Energy Method When a force F undergoes a displacement dx in the same direction i as the force, the work done is du e = F dx If the
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More informationσ = Eα(T T C PROBLEM #1.1 (4 + 4 points, no partial credit)
PROBLEM #1.1 (4 + 4 points, no partial credit A thermal switch consists of a copper bar which under elevation of temperature closes a gap and closes an electrical circuit. The copper bar possesses a length
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More informationChapter 5 Torsion STRUCTURAL MECHANICS: CE203. Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson
STRUCTURAL MECHANICS: CE203 Chapter 5 Torsion Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson Dr B. Achour & Dr Eng. K. Elkashif Civil Engineering Department, University
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationCOURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)
Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationSTRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationProf. B V S Viswanadham, Department of Civil Engineering, IIT Bombay
50 Module 4: Lecture 1 on Stressstrain relationship and Shear strength of soils Contents Stress state, Mohr s circle analysis and Pole, Principal stressspace, Stress pathsin pq space; MohrCoulomb failure
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationFor more Stuffs Visit Owner: N.Rajeev. R07
Code.No: 43034 R07 SET1 JAWAHARLAL NEHRU TECHNOLOGICAL UNIVERSITY HYDERABAD II.B.TECH  I SEMESTER REGULAR EXAMINATIONS NOVEMBER, 2009 FOUNDATION OF SOLID MECHANICS (AERONAUTICAL ENGINEERING) Time: 3hours
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationExam paper: Biomechanics
Exam paper: Biomechanics Tuesday August 10th 2010; 9.0012.00 AM Code: 8W020 Biomedical Engineering Department, Eindhoven University of Technology The exam comprises 10 problems. Every problem has a maximum
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationDue Monday, September 14 th, 12:00 midnight
Due Monday, September 14 th, 1: midnight This homework is considering the analysis of plane and space (3D) trusses as discussed in class. A list of MatLab programs that were discussed in class is provided
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationPredicting Deformation and Strain Behavior in Circuit Board Bend Testing
Predicting Deformation and Strain Behavior in Circuit Board Bend Testing by Ronen Aniti ARLCR0693 May 2012 prepared by Science and Engineering Apprenticeship Program George Washington University 2121
More informationModule 4 : Deflection of Structures Lecture 4 : Strain Energy Method
Module 4 : Deflection of Structures Lecture 4 : Strain Energy Method Objectives In this course you will learn the following Deflection by strain energy method. Evaluation of strain energy in member under
More informationRatcheting deformation in thin film structures
Ratcheting deformation in thin film structures Z. SUO Princeton University Work with MIN HUANG, Rui Huang, Jim Liang, Jean Prevost Princeton University Q. MA, H. Fujimoto, J. He Intel Corporation Interconnect
More informationIf the number of unknown reaction components are equal to the number of equations, the structure is known as statically determinate.
1 of 6 EQUILIBRIUM OF A RIGID BODY AND ANALYSIS OF ETRUCTURAS II 9.1 reactions in supports and joints of a twodimensional structure and statically indeterminate reactions: Statically indeterminate structures
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationUnit 15 Shearing and Torsion (and Bending) of Shell Beams
Unit 15 Shearing and Torsion (and Bending) of Shell Beams Readings: Rivello Ch. 9, section 8.7 (again), section 7.6 T & G 126, 127 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering
More information1 Stress and Strain. Introduction
1 Stress and Strain Introduction This book is concerned with the mechanical behavior of materials. The term mechanical behavior refers to the response of materials to forces. Under load, a material may
More informationTHEORY OF PLATES AND SHELLS
THEORY OF PLATES AND SHELLS S. TIMOSHENKO Professor Emeritus of Engineering Mechanics Stanford University S. WOINOWSKYKRIEGER Professor of Engineering Mechanics Laval University SECOND EDITION MCGRAWHILL
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationSect Least Common Denominator
4 Sect.3  Least Common Denominator Concept #1 Writing Equivalent Rational Expressions Two fractions are equivalent if they are equal. In other words, they are equivalent if they both reduce to the same
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationChapter 2 CONTINUUM MECHANICS PROBLEMS
Chapter 2 CONTINUUM MECHANICS PROBLEMS The concept of treating solids and fluids as though they are continuous media, rather thancomposedofdiscretemolecules, is one that is widely used in most branches
More informationElements of Polymer Structure and Viscoelasticity. David M. Parks Mechanics and Materials II February 18, 2004
Elements of Polymer Structure and Viscoelasticity David M. Parks Mechanics and Materials II 2.002 February 18, 2004 Outline Elements of polymer structure Linear vs. branched; Vinyl polymers and substitutions
More informationBME 207 Introduction to Biomechanics Spring 2017
April 7, 2017 UNIVERSITY OF RHODE ISAND Department of Electrical, Computer and Biomedical Engineering BE 207 Introduction to Biomechanics Spring 2017 Homework 7 Problem 14.3 in the textbook. In addition
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More informationFinite Element Method (FEM)
Finite Element Method (FEM) The finite element method (FEM) is the oldest numerical technique applied to engineering problems. FEM itself is not rigorous, but when combined with integral equation techniques
More informationStress Transformation Equations: u = +135 (Fig. a) s x = 80 MPa s y = 0 t xy = 45 MPa. we obtain, cos u + t xy sin 2u. s x = s x + s y.
014 Pearson Education, Inc., Upper Saddle River, NJ. All rights reserved. This material is protected under all copyright laws as they currently 9 7. Determine the normal stress and shear stress acting
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationCIV E 205 Mechanics of Solids II. Course Notes
University of Waterloo Department of Civil Engineering CIV E 205 Mechanics of Solids II Instructor: Tarek Hegazi Room: CPH 2373 G, Ext. 2174 Email: tarek@uwaterloo.ca Course Web: www.civil.uwaterloo.ca/tarek/hegazy205.html
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More information